LMucko/crystallography-open-database huggingface dataset:
Crystal chemistry of the tsumcorite-group minerals. New data on ferrilotharmeyerite, tsumcorite, thometzekite, mounanaite, helmutwinklerite, and a redefinition of gartrellite
Krause, W.; Belendorff, K.; Bernhardt, H. J.; McCammon, C. A.; Effenberger, H.; Mikenda, W.; European Journal of Mineralogy 10 (1998) 179–206; doi:

data_9005326
_publ_section_title
;Crystal chemistry of the tsumcorite-group minerals. New data on
 ferrilotharmeyerite, tsumcorite, thometzekite, mounanaite, helmutwinklerite,
 and a redefinition of gartrellite
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              179
_journal_page_last               206
_journal_volume                  10
_journal_year                    1998
_chemical_compound_source        'Tsumeb mine, Namibia'
_chemical_formula_sum            'As2 Cu Fe H2 O10 Pb'
_chemical_name_mineral           Gartrellite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                67.62
_cell_angle_beta                 69.57
_cell_angle_gamma                70.31
_cell_formula_units_Z            1
_cell_length_a                   5.431
_cell_length_b                   5.642
_cell_length_c                   7.573
_cell_volume                     195.422
_database_code_amcsd             0006711
_exptl_crystal_density_diffrn    5.425
_cod_original_formula_sum        'Pb Fe Cu As2 (O10 H2)'
_cod_database_code               9005326
Crystal chemistry of the tsumcorite-group minerals. New data on ferrilotharmeyerite, tsumcorite, thometzekite, mounanaite, helmutwinklerite, and a redefinition of gartrellite
Krause, W.; Belendorff, K.; Bernhardt, H. J.; McCammon, C. A.; Effenberger, H.; Mikenda, W.; European Journal of Mineralogy 10 (1998) 179–206; doi:

data_9005327
_publ_section_title
;Crystal chemistry of the tsumcorite-group minerals. New data on
 ferrilotharmeyerite, tsumcorite, thometzekite, mounanaite, helmutwinklerite,
 and a redefinition of gartrellite
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              179
_journal_page_last               206
_journal_volume                  10
_journal_year                    1998
_chemical_compound_source        'Tsumeb mine, Namibia'
_chemical_formula_sum            'As2 H2 O10 Pb Zn2'
_chemical_name_mineral           Helmutwinklerite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                70.19
_cell_angle_beta                 69.91
_cell_angle_gamma                69.18
_cell_formula_units_Z            1
_cell_length_a                   5.606
_cell_length_b                   5.610
_cell_length_c                   7.617
_cell_volume                     203.771
_database_code_amcsd             0006712
_exptl_crystal_density_diffrn    5.296
_cod_original_formula_sum        'Pb Zn2 As2 (O10 H2)'
_cod_database_code               9005327
Kentbrooksite from the Kangerdlugssuaq intrusion, East Greenland, a new Mn-REE-Nb-F end-member in a series within the eudialyte group: Description and crystal structure
Johnsen, O.; Grice, J. D.; Gault, R. A.; European Journal of Mineralogy 10 (1998) 207–219; doi:

data_9005328
_publ_section_title
;
 Kentbrooksite from the Kangerdlugssuaq intrusion, East Greenland,
 a new Mn-REE-Nb-F end-member in a series within the eudialyte group:
 Description and crystal structure
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              207
_journal_page_last               219
_journal_volume                  10
_journal_year                    1998
_chemical_compound_source        'Kangerdlugssuaq intrusion, East Greenland'
_chemical_formula_sum
;Al0.13 Ca3.27 Cl0.269 F1.51 Fe0.79 H0.22 Hf0.06 K0.3 Mg0.05 Mn3.68 Na14.479
 Nb0.55 O75.81 Si25.1 Sr0.15 Ti0.23 Y0.42 Zr2.93
;
_chemical_name_mineral           Kentbrooksite
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   14.1686
_cell_length_b                   14.1686
_cell_length_c                   30.0847
_cell_formula_units_Z            3
_cell_volume                     5230.343
_database_code_amcsd             0006713
_exptl_crystal_density_diffrn    2.927
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum
;Ca3.27 Mn3.68 Na14.479 Fe.79 Al.13 Mg.05 Nb.55 Zr2.93 Ti.23 Si25.1 Y.42 K.3
 Sr.15 Hf.06 O75.81 F1.51 Cl.269 H.22
;
_cod_database_code               9005328
An in situ study of the edingtonite dehydration process from X-ray synchrotron powder diffraction Sample: 310 K
Stahl, K.; Hanson, J. C.; European Journal of Mineralogy 10 (1998) 221–228; doi:

data_9005329
_publ_section_title
;
 An in situ study of the edingtonite dehydration process from
 X-ray synchrotron powder diffraction
 Sample: 310 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              221
_journal_page_last               228
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Al2 Ba0.9 Ca0.1 H3.809 O13.08 Si3'
_chemical_name_mineral           Edingtonite
_space_group_IT_number           18
_symmetry_space_group_name_Hall  'P 2 2ab'
_symmetry_space_group_name_H-M   'P 21 21 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.5374
_cell_length_b                   9.6127
_cell_length_c                   6.5233
_cell_volume                     598.057
_database_code_amcsd             0006714
_exptl_crystal_density_diffrn    2.660
_cod_original_formula_sum        '(Ba.9 Ca.1) Al2 Si3 O13.08 H3.809'
_cod_database_code               9005329
An in situ study of the edingtonite dehydration process from X-ray synchrotron powder diffraction Sample: 396 K
Stahl, K.; Hanson, J. C.; European Journal of Mineralogy 10 (1998) 221–228; doi:

data_9005330
_publ_section_title
;
 An in situ study of the edingtonite dehydration process from
 X-ray synchrotron powder diffraction
 Sample: 396 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              221
_journal_page_last               228
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Al2 Ba0.9 Ca0.1 H3.809 O12.46 Si3'
_chemical_name_mineral           Edingtonite
_space_group_IT_number           18
_symmetry_space_group_name_Hall  'P 2 2ab'
_symmetry_space_group_name_H-M   'P 21 21 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.4903
_cell_length_b                   9.5690
_cell_length_c                   6.5290
_cell_volume                     592.916
_database_code_amcsd             0006715
_exptl_crystal_density_diffrn    2.627
_cod_original_formula_sum        '(Ba.9 Ca.1) Al2 Si3 O12.46 H3.809'
_cod_database_code               9005330
An in situ study of the edingtonite dehydration process from X-ray synchrotron powder diffraction Sample: 451 K
Stahl, K.; Hanson, J. C.; European Journal of Mineralogy 10 (1998) 221–228; doi:

data_9005331
_publ_section_title
;
 An in situ study of the edingtonite dehydration process from
 X-ray synchrotron powder diffraction
 Sample: 451 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              221
_journal_page_last               228
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Al2 Ba0.9 Ca0.1 H3.809 O12.04 Si3'
_chemical_name_mineral           Edingtonite
_space_group_IT_number           18
_symmetry_space_group_name_Hall  'P 2 2ab'
_symmetry_space_group_name_H-M   'P 21 21 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.4393
_cell_length_b                   9.5089
_cell_length_c                   6.5042
_cell_volume                     583.800
_database_code_amcsd             0006716
_exptl_crystal_density_diffrn    2.630
_cod_original_formula_sum        '(Ba.9 Ca.1) Al2 Si3 O12.04 H3.809'
_cod_database_code               9005331
An in situ study of the edingtonite dehydration process from X-ray synchrotron powder diffraction Sample: 643 K
Stahl, K.; Hanson, J. C.; European Journal of Mineralogy 10 (1998) 221–228; doi:

data_9005332
_publ_section_title
;
 An in situ study of the edingtonite dehydration process from
 X-ray synchrotron powder diffraction
 Sample: 643 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              221
_journal_page_last               228
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Al2 Ba0.9 Ca0.1 H3.809 O10.68 Si3'
_chemical_name_mineral           Edingtonite
_space_group_IT_number           18
_symmetry_space_group_name_Hall  'P 2 2ab'
_symmetry_space_group_name_H-M   'P 21 21 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.3758
_cell_length_b                   9.4097
_cell_length_c                   6.5377
_cell_volume                     576.779
_database_code_amcsd             0006717
_exptl_crystal_density_diffrn    2.537
_cod_original_formula_sum        '(Ba.9 Ca.1) Al2 Si3 O10.68 H3.809'
_cod_database_code               9005332
Mossbauer spectroscopy and Rietveld refinement on synthetic ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside Sample: Di#S2
Redhammer, G. J.; European Journal of Mineralogy 10 (1998) 439–452; doi:

data_9005333
_publ_section_title
;
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: Di#S2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              439
_journal_page_last               452
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Ca Mg O6 Si2'
_chemical_name_mineral           Diopside
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.882
_cell_angle_gamma                90
_cell_length_a                   9.7483
_cell_length_b                   8.9246
_cell_length_c                   5.2505
_cell_formula_units_Z            4
_cell_volume                     439.355
_database_code_amcsd             0006718
_exptl_crystal_density_diffrn    3.274
_cod_original_formula_sum        'Ca Mg Si2 O6'
_cod_database_code               9005333
Mossbauer spectroscopy and Rietveld refinement on synthetic ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside Sample: fts6/#2
Redhammer, G. J.; European Journal of Mineralogy 10 (1998) 439–452; doi:

data_9005334
_publ_section_title
;
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts6/#2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              439
_journal_page_last               452
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Ca Fe0.13 Mg0.943 O6 Si1.927'
_chemical_name_mineral           Diopside
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.936
_cell_angle_gamma                90
_cell_length_a                   9.7433
_cell_length_b                   8.9410
_cell_length_c                   5.2511
_cell_formula_units_Z            4
_cell_volume                     439.869
_database_code_amcsd             0006719
_exptl_crystal_density_diffrn    3.328
_cod_original_formula_sum        'Ca Mg.943 Fe.13 Si1.927 O6'
_cod_database_code               9005334
Mossbauer spectroscopy and Rietveld refinement on synthetic ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside Sample: fts10/#2
Redhammer, G. J.; European Journal of Mineralogy 10 (1998) 439–452; doi:

data_9005335
_publ_section_title
;
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts10/#2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              439
_journal_page_last               452
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Ca Fe0.205 Mg0.895 O6 Si1.9'
_chemical_name_mineral           Diopside
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.890
_cell_angle_gamma                90
_cell_length_a                   9.7600
_cell_length_b                   8.9236
_cell_length_c                   5.2670
_cell_formula_units_Z            4
_cell_volume                     441.198
_database_code_amcsd             0006720
_exptl_crystal_density_diffrn    3.352
_cod_original_formula_sum        'Ca Mg.895 Fe.205 Si1.9 O6'
_cod_database_code               9005335
Mossbauer spectroscopy and Rietveld refinement on synthetic ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside Sample: fts10/#3
Redhammer, G. J.; European Journal of Mineralogy 10 (1998) 439–452; doi:

data_9005336
_publ_section_title
;
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts10/#3
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              439
_journal_page_last               452
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Ca Fe0.194 Mg0.906 O6 Si1.9'
_chemical_name_mineral           Diopside-ferrian
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.886
_cell_angle_gamma                90
_cell_length_a                   9.7578
_cell_length_b                   8.9226
_cell_length_c                   5.2639
_cell_formula_units_Z            4
_cell_volume                     440.798
_database_code_amcsd             0006721
_exptl_crystal_density_diffrn    3.350
_cod_original_formula_sum        'Ca Mg.906 Fe.194 Si1.9 O6'
_cod_database_code               9005336
Mossbauer spectroscopy and Rietveld refinement on synthetic ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside Sample: fts15/#2
Redhammer, G. J.; European Journal of Mineralogy 10 (1998) 439–452; doi:

data_9005337
_publ_section_title
;
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts15/#2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              439
_journal_page_last               452
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Ca Fe0.267 Mg0.857 O6 Si1.876'
_chemical_name_mineral           Diopside-ferrian
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.889
_cell_angle_gamma                90
_cell_length_a                   9.7646
_cell_length_b                   8.9200
_cell_length_c                   5.2709
_cell_formula_units_Z            4
_cell_volume                     441.556
_database_code_amcsd             0006722
_exptl_crystal_density_diffrn    3.377
_cod_original_formula_sum        'Ca Mg.857 Fe.267 Si1.876 O6'
_cod_database_code               9005337
Mossbauer spectroscopy and Rietveld refinement on synthetic ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside Sample: fts20/#2
Redhammer, G. J.; European Journal of Mineralogy 10 (1998) 439–452; doi:

data_9005338
_publ_section_title
;
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts20/#2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              439
_journal_page_last               452
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Ca Fe0.445 Mg0.805 O6 Si1.75'
_chemical_name_mineral           Diopside-ferrian
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.881
_cell_angle_gamma                90
_cell_length_a                   9.7724
_cell_length_b                   8.9176
_cell_length_c                   5.2837
_cell_formula_units_Z            4
_cell_volume                     442.881
_database_code_amcsd             0006723
_exptl_crystal_density_diffrn    3.444
_cod_original_formula_sum        'Ca Mg.805 Fe.445 Si1.75 O6'
_cod_database_code               9005338
Mossbauer spectroscopy and Rietveld refinement on synthetic ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside Sample: fts30/#2
Redhammer, G. J.; European Journal of Mineralogy 10 (1998) 439–452; doi:

data_9005339
_publ_section_title
;
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts30/#2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              439
_journal_page_last               452
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Ca Fe0.597 Mg0.733 O6 Si1.67'
_chemical_name_mineral           Diopside-subsilisic
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.883
_cell_angle_gamma                90
_cell_length_a                   9.7844
_cell_length_b                   8.9132
_cell_length_c                   5.2989
_cell_formula_units_Z            4
_cell_volume                     444.476
_database_code_amcsd             0006724
_exptl_crystal_density_diffrn    3.499
_cod_original_formula_sum        'Ca Mg.733 Fe.597 Si1.67 O6'
_cod_database_code               9005339
Mossbauer spectroscopy and Rietveld refinement on synthetic ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside Sample: fts40/#1
Redhammer, G. J.; European Journal of Mineralogy 10 (1998) 439–452; doi:

data_9005340
_publ_section_title
;
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts40/#1
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              439
_journal_page_last               452
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Ca Fe0.759 Mg0.641 O6 Si1.2'
_chemical_name_mineral           Diopside-subsilisic
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.856
_cell_angle_gamma                90
_cell_length_a                   9.8007
_cell_length_b                   8.9002
_cell_length_c                   5.3214
_cell_formula_units_Z            4
_cell_volume                     446.515
_database_code_amcsd             0006725
_exptl_crystal_density_diffrn    3.388
_cod_original_formula_sum        'Ca Mg.641 Fe.759 Si1.2 O6'
_cod_database_code               9005340
Crystal-structure refinement of synthetic Fe- and Mg-staurolite by Rietveld analysis of X-ray powder-diffraction data Sample: Mg-staurolite synthesized at 25 kbar
Koch-Muller M; Kahlenberg, V.; Bubenick, W.; Gottschalk, M.; European Journal of Mineralogy 10 (1998) 453–460; doi:

data_9005341
_publ_section_title
;
 Crystal-structure refinement of synthetic Fe- and Mg-staurolite by
 Rietveld analysis of X-ray powder-diffraction data
 Sample: Mg-staurolite synthesized at 25 kbar
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              453
_journal_page_last               460
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Al4.39 Mg0.9 O12 Si1.96'
_chemical_name_mineral           Staurolite
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2c'
_symmetry_space_group_name_H-M   'C c m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8791
_cell_length_b                   16.5425
_cell_length_c                   5.6329
_cell_formula_units_Z            4
_cell_volume                     734.192
_database_code_amcsd             0006726
_exptl_crystal_density_diffrn    3.504
_exptl_crystal_pressure_history  'synthesized at 25 kbar'
_cod_original_formula_sum        'Mg.9 Al4.39 Si1.96 O12'
_cod_database_code               9005341
Crystal-structure refinement of synthetic Fe- and Mg-staurolite by Rietveld analysis of X-ray powder-diffraction data Sample: Fe-staurolite synthesized at 25 kbar
Koch-Muller M; Kahlenberg, V.; Bubenick, W.; Gottschalk, M.; European Journal of Mineralogy 10 (1998) 453–460; doi:

data_9005342
_publ_section_title
;
 Crystal-structure refinement of synthetic Fe- and Mg-staurolite by
 Rietveld analysis of X-ray powder-diffraction data
 Sample: Fe-staurolite synthesized at 25 kbar
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              453
_journal_page_last               460
_journal_volume                  10
_journal_year                    1998
_chemical_formula_sum            'Al2.305 Fe0.44 O6 Si0.95'
_chemical_name_mineral           Staurolite
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2c'
_symmetry_space_group_name_H-M   'C c m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8719
_cell_length_b                   16.6231
_cell_length_c                   5.6583
_cell_formula_units_Z            8
_cell_volume                     740.419
_database_code_amcsd             0006727
_exptl_crystal_density_diffrn    3.758
_exptl_crystal_pressure_history  'synthesized at 25 kbar'
_cod_original_formula_sum        'Fe.44 Al2.305 Si.95 O6'
_cod_database_code               9005342